## Synthesis and post-annealing effects of alkaline-metal-ethylenediamine-intercalated superconductors Ax (C2H8N2) Fe2- Se2 ( y z A = Li, Na) with T c = 45 K

Takashi Noji, Takehiro Hatakeda, Shohei Hosono, Takayuki Kawamata, Masatsune Kato, Yoji Koike

Department of Applied Physics, Graduate School of Engineering, Tohoku University,

6-6-05 Aoba, Aramaki, Aoba-ku, Sendai 980-8579, Japan

New iron-based intercalation superconductors Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) with T c = 45 K have successfully been synthesized via intercalation of dissolved alkaline metal in ethylenediamine.  The c -axis  lengths  of Ax (C2H8N2) Fe2y z Se2  ( A =  Li,  Na)  are  20.74(7)  Å  and 21.9(1) Å, respectively, and are about 50 % larger than that of K Fe2 x Se2, indicating that not only alkaline  metal  but  also  ethylenediamine  is  intercalated  between  the  Se-Se  layers  of  FeSe.  It seems  that  the  highT c of Ax (C2H8N2) Fe2y z Se2  ( A =  Li, Na)  is  caused  by  the  possible two-dimensional electronic structure due to the large c -axis length. Through the post-annealing in an evacuated glass tube, it has been found that T c decreases with increasing post-annealing temperature and that deintercalation of EDA from the as-intercalated sample takes place at low temperatures below 250 ℃ .

Keywords: superconductivity, intercalation, FeSe, etylenediamine, alkaline metal

## 1. Introduction

The  superconducting  transition  temperature, T c , of  the  iron-based  chalcogenide superconductor  FeSe  is  only  8  K  [1],  but  dramatically  increases  up  to  ~37  K  by  the application  of  high  pressure  [2].  The  successful  synthesis  of  potassium-intercalated KxFe2-ySe2  with T c ~31  K  at  ambient  pressure  was  an  exciting  breakthrough  [3]. Recently,  it has been  reported  that the intercalation into FeSe  of  alkaline and alkaline-earth metals in liquid ammonia yields a variety of compounds with significantly enhanced T c 's of 40 - 46 K [4 - 6]. The c-axis length of Li0.9Fe2Se2(NH3)0.5 with T c =  44  K is 16.518 Å [5] and larger than 14.0367 Å in K Fe2Se2 [3], indicating x that not only lithium but also ammonia is intercalated. Moreover, it has been reported that  lithium-  and  pyridine-intercalated  Li (C5H5N) Fe2x y z Se2  exhibits  superconductivity with T c =  45  K  and that post-annealing of the intercalated sample drastically expands the c -axis  length  from  16.0549  Å  to  23.09648  Å  and  increases  the  superconducting shielding volume fraction [7].

Here, we report on the successful synthesis of new superconductors Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) with T c = 45 K via intercalation of dissolved alkaline metal in ethylenediamine (EDA), C2H8N2. Post-annealing effects on the crystal structure and superconductivity are also discussed.

## 2. Experimenta l

Polycrystalline samples of FeSe were prepared by the solid-state reaction method. Starting materials were powders of Fe and Se, which were weighted stoichiometrically, mixed  thoroughly  and  pressed  into  pellets.  The  pellets  were  sealed  in  an  evacuated quartz tube and heated at 800 ℃ for 40 h. The obtained pellets of FeSe were pulverized into  powder  to  use  for  the  intercalation.  Dissolved  alkaline  metal  in  EDA  was intercalated into the powdery FeSe as follows. An appropriate amount of the powdery FeSe was placed in a beaker filled with 0.2 M solution of pure lithium or sodium metal dissolved  in  EDA.  All  the  process  was  performed  in  an  argon-filled  glove  box. Post-annealing of as-intercalated samples was carried out at 100 - 500 ℃ for 60 h in an evacuated  glass  tube.  Both  FeSe  and  the  intercalated  samples  were  characterized  by powder x-ray diffraction using Cu Kα radiation. For the intercalated samples, an airtight sample  holder  was  used.  In  order  to  observe  the  superconducting  transition,  the magnetic susceptibility, χ , was measured using a superconducting quantum interference device (SQUID) magnetometer. Measurements of the electrical resistivity, ρ , were also carried out by the standard dc four-probe method. For the ρ measurements, as-intercalated  powdery  samples  were  pressed  into  pellets.  Then,  the  pellets  were sintered  at  200 ℃ for  20  h  in  an  evacuated  glass  tube.  Thermogravimetric  (TG) measurements were performed in flowing  gas of argon, using a  commercial  analyzer (SII Nano Technology Inc., EXSTAR DSC7020).

## 3. Results and discussion

Figure  1  shows  powder  x-ray  diffraction  patterns  of  as-intercalated  samples  of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na). The broad peak around 2 θ = 20° is due to the airtight sample holder. Although there are unknown peaks, most of sharp Bragg peaks are due to the intercalation compound of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) and the host compound of FeSe, so that they are able to be indexed based on the ThCr2Si2-type and PbO-type structures, respectively. Therefore, it is found that alkaline metal and EDA are partially intercalated  into  FeSe,  while  there  remains  a  non-intercalated  region  of  FeSe  in  the

Fig.  1.  Powder  x-ray  diffraction  patterns  of  as-intercalated  samples  consisting  of A x (C H N ) Fe 2 8 2 y 2z Se  ( 2 A = Li, Na) and FeSe using Cu K  radiation. Indexes without and α with  asterisk  are  based  on  the  ThCr Si -type  and  PbO-type  structures,  respectively. 2 2 Peaks marked by ▼ are unknown.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0346v1-figure-f8c134e2-9602-4c90-9749-93b57e4e4fc4.jpg)

samples. The lattice constants of Li (C2H8N2) Fe2x y z Se2 are calculated to be a = 3.458(6) Å and c = 20.74(7) Å. The c-axis length of Na (C2H8N2) Fe2x y z Se2 is 21.9(1) Å. Since the unit  cell  of Ax (C2H8N2) Fe2y z Se2  ( A =  Li,  Na)  includes  two  Fe  layers,  the  distance between the neighboring Fe layers is 10.37(4) Å and 10.95(5) Å, respectively, and much larger  than  5.515(1)  Å  of  FeSe.  Taking  into  account  our  previous  results  that  the intercalation of only lithium into Fe(Se,Te) has neither effect on the superconductivity nor crystal structure [8], it is concluded that not only lithium or sodium but also EDA has been intercalated between the Se-Se layers of FeSe.

Figure  2  shows  the  temperature  dependence  of χ in  a  magnetic  field  of  10  Oe  on zero-field cooling (ZFC) and on field cooling (FC) for as-intercalated powdery samples. The first T c is  observed  at  45  K  and  the second T c is  at  8  K.  Taking  into  account  the powder  x-ray diffraction results, it is concluded that the first is due to bulk superconductivity of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na), while the second is due to that of the non-intercalated region of FeSe. The inset shows the temperature dependence of ρ for  the  sintered  (200 ℃ , 20  h)  pellet  sample.  Although  the  as-intercalated  sample pelletized simply at room temperature did not show zero resistivity, it is found that the resistivity  of  the  sintered  pellet  sample  starts  to  decrease  at  43  K  with  decreasing temperature and reaches zero at 18 K. Since the intercalation of only lithium does not increase T c [8], it seems that the highT c of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) is caused by the possible two-dimensional electronic structure due to the large c-axis length.

Figure 3 shows the TG curve on heating up to 900 ℃ at the rate of 1 ℃ /min for the as-intercalated  powdery  sample.  Three  steps  of  mass  loss  are  observed;  2.9  %  loss below 100 ℃ , 11.3 % loss between 100 and 200 ℃ , and large loss above 450 ℃ .

Fig. 3. Thermogravimetric (TG) curve on heating at the  rate  of  1 ℃ /min  for  the  as-intercalated  powdery sample consisting of Li (C2H8N2) Fe2x y z Se2 and FeSe.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0346v1-figure-63660f43-ee28-47f5-b232-19c1cc36cb7d.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0346v1-figure-61b05cff-e030-441d-8a29-7c33adf49d50.jpg)

Fig. 2. Temperature dependence of the magnetic susceptibility, χ , in a magnetic field of 10 Oe on  zero-field  cooling  (ZFC)  and  field  cooling  (FC)  for  as-intercalated  powdery  samples consisting  of Ax (C2H8N2) Fe2y z Se2  ((a) A =  Li,  (b) A =  Na)  and  FeSe.  The  inset  shows  the temperature dependence of the electrical resistivity, ρ ,  for  the  sintered  (200 ℃ ,  20  h)  pellet sample consisting of Li (C2H8N2) Fe2x y z Se2 and FeSe.

Figure  4  shows  powder  x-ray  diffraction  patterns  of  the  as-intercalated  sample  and samples  post-annealed  at  various  temperatures  for  60  h.  For  samples  post-annealed below 200 ℃ , diffraction peaks of Li (C2H8N2) Fe2x y z Se2 remain. For samples post-annealed  at  250 ℃ and  300 ℃ ,  only  peaks  due  to  FeSe  are  observed,  and  these peaks disappear for the sample post-annealed at 500 ℃ . Accordingly, the first step of the TG curve below 100 ℃ may be due to desorption of EDA on the surface of grains. The second step between 100 and 220 ℃ is  due  to  deintercalation  of  EDA.  The third step above 500 ℃ may be due to unknown products including iron.

Figure 5 shows the temperature dependence of χ in a magnetic field of 10 Oe on ZFC and FC for as-intercalated and post-annealed (100 - 500 ℃ , 60 h) powdery samples. The T c of  Li (C H8N2) Fe2x 2 y z Se2 decreases  with  increasing  post-annealing  temperature.  For samples post-annealed at 250 ℃ and 300 ℃ , only the superconducting transition of FeSe is  observed,  and  the  transition  also  disappears  for  the  sample  post-annealed  at  500 ℃ . These results are in good correspondence to the results of x-ray diffraction.

Fig. 4. Powder x-ray diffraction patterns of as-intercalated and post-annealed (100 - 500 ℃ , 60 h) samples using Cu K  radiation. Indexes without and α with asterisk are based on the ThCr Si -type and 2 2 PbO-type structures, respectively.    Peaks marked by▼ are unknown.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0346v1-figure-d25ab3e5-a66c-40d7-b617-582952ed3202.jpg)

Fig.  5.  Temperature  dependence  of  the  magnetic  susceptibility, χ ,  in  a  magnetic  field  of  10  Oe  on zero-field cooling (ZFC) and field cooling (FC) for as-intercalated and post-annealed (100 - 500 ℃ , 60 h) powdery samples consisting of Li (C2H8N2) Fe2x y z Se2 and FeSe.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0346v1-figure-48a2ddfb-55d0-47f7-94c2-77a0e1a8b3a7.jpg)

Finally, Fig. 6 shows the maximum Tc 's of FeSe-based superconductors obtained so far at ambient pressure as a function of the distance between the neighboring Fe layers. Interestingly, Tc increases monotonically with increasing such distance and is saturated at about 45 K above 9 Å.

Fig. 6. Relation between the maximum T c and the distance of the neighbouring Fe layers of FeSe-based superconductors.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0346v1-figure-cbbe4aff-0124-4d31-8d1b-9a38ffd3449c.jpg)

## 4. Summary

We have succeeded in synthesizing new intercalation compounds Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) via intercalation of dissolved alkaline metal in EDA. Although the samples include non-intercalated regions of FeSe, the c -axes of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) have drastically expanded to be 20.74(7) and 21.9(1) Å,  respectively,  indicating  that  not  only  alkaline  metal  but  also  EDA  is  intercalated between the Se-Se layers of FeSe. Bulk superconductivity has been observed below 45 K in the χ measurements of as-intercalated samples of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na). Moreover, zero resistivity has been observed below 18 K for the sintered pellet sample of Li (C2H8N2) Fe2x y z Se2. It seems that the highT c of Ax (C2H8N2) Fe2y z Se2 ( A = Li, Na) is caused  by  the  possible  two-dimensional  electronic  structure  due  to  the  large  c-axis length. Through the post-annealing in an evacuated glass tube, it has been found that T c decreases with increasing post-annealing temperature and that deintercalation of EDA from the as-intercalated sample takes place at low temperatures below 250 ℃ and that FeSe remains at temperatures around 400 ℃ .  It  has  also  turned  out  that  the  maximum T c 's of FeSe-based  superconductors  rise with increasing distance between  the neighboring Fe layers and are saturated at about 45 K above 9 Å.

## References

- [1] F.-C. Hsu, J.-Y. Luo, K.-W. Yeh, T.-K. Chen, T.-W. Huang, P. M. Wu, Y.-C. Lee, Y.-L. Huang, Y.-Y. Chu, D.-C. Yan, and M.-K. Wu, Proc. Natl. Acad. Sci. U.S.A 105 (2008) 14262 - 14264.
- [2] S. Margadonna, Y. takabayashi, Y. Ohishi, Y. Mizuguchi, Y. Takano, T. Kagayama. T. Nakagawa, M. Takata, and K. Prassides, Phys. Rev. B 80 (2009) 064506/1 - 6.
- [3] J. Guo, S. Jin, G. Wang, S. Wang, K. Zhu, T. Zhou, M. He, and X. Chen, Phys. Rev. B 82 (2010) 180520(R)/1 - 4.
- [4] T. P. Ying, X. L. Chen, G. Wang, S. F. Jin, T. T. Zhou, X. F. Lai, H. Zhang, and W. Y. Wang, Sci. Rep. 2 (2012) 426/1 - 7.
- [5]  E.-W.  Scheidt,  V.  R.  Hathwar,  D.  Schmitz,  A.  Dunbar,  W.  Scherer,  F.  Mayr,  V. Tsurkan, J. Deisenhofer, and A.Loidl, Eur. Phys. J. B 85 (2012) 279/1 - 5.
- [6] M. Burrard-Lucas, D. G. Free, S. J. Sedlmaier, J. D. Wright, S. J. Cassidy, Y. Hara, A. J. Corkett, T. Lancaster, P. J. Baker, S. J. Blundell, and S. J. Clarke, Nat. Mater. 12 (2013) 15 - 19.
- [7] A. Krzton-Maziopa, E. V. Pomjakushina, V. Y. Pomjakushin, F. Rohr, A. Schilling, and K. Conder, J. Phys.: Condens. Matter 24 (2012) 382202/1 - 6.
- [8] H. Abe, T. Noji, M. Kato, and Y. Koike, Physica C 470 (2010) S487 - S488.
- [9] A. Krzton-Maziopa, Z. Shermadini, E. Pomjakushina, V. Pomjakushin, M. Bendele, A. Amato, R. Khasanov, H. Luetkens, and K. Conder, J. Phys.: Condens. Matter 23 (2011) 052203/1 - 4.
- [10] A. F. Wang, J. J. Ying, Y. J. Yan, R. H. Liu, X. G. Luo, Z. Y. Li, X. F. Wang, M. Zhang, G. J. Ye, P. Cheng, Z. J. Xiang, and X. H. Chen, Phys. Rev. B 83 (2011) 060512(R)/1 - 4.
- [11] K.-W. Yeh, T.-W. Huang, Y.-L. Huang, T.-K. Chen, F.-C. Hsu, P. M. Wu, Y.-C. Lee, Y.-Y. Chu, C.-L. Chen, J.-Y. Luo, D.-C. Yan, and M.-K. Wu: Europhys. Lett. 84 (2008) 37002/1 - 4.
- [12] A. -M. Zhang, T. -L. Xia, K. Liu, W. Tong, Z. -R. Yang, and Q. -M. Zhang, Sci. Rep. 3 (2013) 1216/1 - 5.
Takashi Noji Takehiro Hatakeda Shohei Hosono Takayuki Kawamata Masatsune Kato Yoji Koike
Synthesis and post-annealing effects of alkaline-metal-ethylenediamine-intercalated superconductors Ax(C2H8N2)yFe2-zSe2 (A = Li, Na) with Tc = 45 K
New iron-based intercalation superconductors Ax(C2H8N2)yFe2-zSe2 (A = Li, Na)
with Tc = 45 K have successfully been synthesized via intercalation of
dissolved alkaline metal in ethylenediamine. The c-axis lengths of
Ax(C2H8N2)yFe2-zSe2 (A = Li, Na) are 20.74(7) {\AA} and 21.9(1) {\AA},
respectively, and are about 50 % larger than that of KxFe2Se2, indicating that
not only alkaline metal but also ethylenediamine is intercalated between the
Se-Se layers of FeSe. It seems that the high-Tc of Ax(C2H8N2)yFe2-zSe2 (A = Li,
Na) is caused by the possible two-dimensional electronic structure due to the
large c-axis length. Through the post-annealing in an evacuated glass tube, it
has been found that Tc decreases with increasing post-annealing temperature and
that deintercalation of EDA from the as-intercalated sample takes place at low
temperatures below 250 {\deg}C.